three dimensional simulation of coextrusion in a · die. this finite element mesh is not modified...
Embed Size (px)
Three Dimensional Simulation of Coextrusion in aComplex Profile DiePrint(10) » 3D Simulation of the Fluted Mixer Element Behavior » Prediction of Secondary Flows in NonCircular Ducts Usingthe Radial Functions Method » Three Dimensional Simulation of Coextrusion in a Complex Profile Die
Three Dimensional Simulation of Coextrusion in aComplex Profile DieMahesh GuptaMichigan Technological University Plastic Flow, LLCHoughton, MI 49931 Houghton, MI 49931
AbstractMesh partitioning technique is used to simulate bilayer coextrusion in a complex profile extrusion die. Mesh partitioningtechnique allows coextrusion simulation without changing the finite element mesh as the interface between theadjacent polymer layers is changed during a coextrusion simulation. Since the finite element mesh in the die remainsfixed during the simulation, the mesh partitioning technique allows coextrusion simulation even in highly complicatedprofile dies. Effect of polymer viscosity on interface shape, velocity, pressure, shear rate, and residence timedistribution in a profile coextrusion die is analyzed. It is found that polymer viscosity has significant effect on theinterface shape, velocity, pressure, and shear rate, but only a minor effect on the residence time distribution in the die.
IntroductionCoextrusion, which involves simultaneous extrusion of several different polymers through a die to form a singlemultilayered product, combines the functionalities and benefits of several polymers into a single product . Despitethis inherent advantage of coextrusion, growth of coextrusion market has been slowed down by the complexity ofcoextrusion die design. Depending upon the rheology of polymers used for coextrusion, the polymers in various layersmay get redistributed as they flow through the die such that the distribution of various polymers at the inlet and at theexit of the die may be quite different. Because of this redistribution of polymer layers, finding a die geometry which willgive the required layer distribution in the final product can be extremely difficult.
Coextrusion dies are currently designed using a “trial and error” approach. This repetitive approach is not only highlytimeconsuming and costly, but also requires highly experienced engineers and rarely provides an optimum die design.Therefore, a coextrusion simulation software, which can accurately predict the shape of the interface between differentpolymer layers, is an excellent designaide for a coextrusion die designer. A coextrusion software not onlytremendously simplifies the coextrusion die design process, the software can also be exploited for a proper selection ofthe material in different layers and for optimization of the processing conditions.
Coextrusion Simulation EquationsFor simulation of a multilayer flow of polymers during coextrusion, the velocity and stresses are required to becontinuous across the interface between the adjacent polymer layers . That is,
where I contains all finite elements nodes on the interface, v(vector)i(1) and τ~i
(1) are the velocities and stresses on
one side of the interface, with v(vector)i(2) and τ~i
(2) being the velocities and stresses on the other side of theinterface. Besides the continuity of velocity and stress, coextrusion simulation requires enforcement of the nocross
flow condition at the interface. That is, the velocity component normal to the interface must be zero at all interfacenodes:
where v(vector)i is the velocity, and n(vector)i is the unit vector perpendicular to the interface.
Mesh Partitioning TechniqueIn most threedimensional simulations of coextrusion reported in the literature, finite element mesh is modified aftereach flow simulation iteration, such that the interelement boundaries coincide with the interface between adjacentlayers of different polymers . Such an approach using an interfacematched finite element mesh can only beemployed for simulating a twodimensional system or a simple threedimensional system such as a rectangular die. Forreallife coextrusion systems, with complex threedimensional die channel geometry, repeated generation andmodification of interfacematched finite element meshes is impractical.
In the present work, polyXtrue software  was used to simulate the flow in a bilayer profile coextrusion die. In thissoftware a threedimensional mesh of tetrahedral finite elements is generated over the complete flow domain in thedie. This finite element mesh is not modified or regenerated at any stage during coextrusion simulation. Thereby,allowing simulation of even highly complex coextrusion systems.
In the coextrusion software used in this work, the interface between adjacent layers of different polymers isrepresented by a surface mesh of linear triangular finite elements. However, the surface mesh of triangular elementson the interface and the threedimensional mesh of tetrahedral elements in the coextrusion die are completelyindependent of each other. This decoupling between the two finiteelement meshes is possible because in the meshpartitioning technique for coextrusion simulation, the interface between adjacent polymer layers is not required tomatch with the interelement boundaries in the threedimensional mesh of tetrahedral finite elements. Instead, in thesoftware used in this work, the interface is allowed to pass through the interior of the tetrahedral finite elements in thethreedimensional mesh.
In the mesh partitioning technique for coextrusion simulation, the tetrahedral elements which are intersected by themesh of triangular elements on the interface are partitioned into two threedimensional finite elements. When a twodimensional plane intersects a tetrahedral finite element, it leads to one of the following combinations of two finiteelements.o One tetrahedral and one prismatic element (Fig. 1 a),o Two tetrahedral elements (Fig. 1 b),o One pyramidal and one tetrahedral element (Fig. 1 c)o Two prismatic elements (Fig. 1 d).In the coextrusion software used, each of the tetrahedral elements which are intersected by the interface betweenadjacent polymer layers is replaced by one of these four combinations of the two finite elements.
Prediction of Interface ShapeThe shape of the interface between adjacent polymer layers is defined by the nocrossflow boundary condition (Eqn.3). In the coextrusion software used in this work, a weighted residual form of Eqn. 3 is solved to predict the interfaceshape .
where Is is the space of weighting functions (same as the shape functions) on the interface and Γ denotes the interfacesurface.
In our earlier publication  on coextrusion simulation for simpler extrudate shapes, an initial estimate of the interfaceshape had to be specified as an input to the coextrusion software. Starting with the initial estimate of the interfaceshape, the earlier version of the software then accurately predicted the interface shape between the adjacent polymerlayers. For complicated profile coextrusion dies, such as the die analyzed in this work, it is difficult to determine theinitial estimate of the interface between the adjacent polymer layers. Therefore, in the current version of the polyXtruesoftware, using the streamlines for the flow simulation in the previous iteration, an initial estimate of the interface
between the adjacent polymer layers is automatically determined by the software. This initial estimate of the interfaceshape obtained from the streamlines for the previous flow iteration is then updated according to the predictions fromthe weighted residual form of the nocrossflow condition (Eqn. 4).
ResinsThe generalized Newtonian formulation for an inertialess, incompressible flow with shearthinning viscosity was usedfor the coextrusion simulations. To simulate a multilayer flow in coextrusion dies, two different grades of lowdensitypolyethylene (LDPE) were used in this work. The shear viscosity data at 200oC for the two grades of LDPE is shown inFig. 2. Experimental data from reference  (Fig. 2) was used to obtain the parameters for the Cross model (Table 1).
Fig. 2 also shows the viscosity curves based upon the Cross model parameters given in Table 1.
Results and DiscussionThe geometry of the complex profile die analyzed, and the mesh of tetrahedral elements used for coextrusionsimulation is shown in Fig. 3. Most of the extruded profile (substrate) is made of one polymer, but it has a thin caplayer on the top wall. As shown in Fig. 4, the cap layer also wraps around the vertical tab on the left side of the part.For substrate of the profile the polymer enters along the axial direction into a circular channel which is graduallytransformed into the profile shape. The cap layer enters through a circular channel on top, which is perpendicular tothe die axis. In order to distribute the polymer from the circular channel to the thin cap layer, the circular channel isfollowed by two distribution channels. Both distribution channels have circular crosssections, and are connected by achannel with uniform narrow opening. Because of the narrow channel between the two distribution channels, thepolymer first flows along the transverse direction and is distributed in the first distribution channel before it enters intothe second distribution channel. The second distribution channel is connected to the entrance of the cap layer in thedie, again by a narrow channel which further distributes the polymer in the second distribution channel before thepolymer uniformly reaches the contact line where the cap layer meets the substrate for the first time.
The flow in the bilayer profile die was simulated for the following three different combinations of LDPEA and LDPEDin the substrate and the cap layer.
Substrate | Cap layerLDPEA | LDPEALDPEA | LDPEDLDPED | LDPEA
For these three combinations of LDPEA and LDPED, the velocities at the circular entrances of the substrate and caplayer were 0.1 cm/s and 1.5 cm/s, respectively. These values of entrance velocities were used so that the velocities ofthe two polymers are similar when the two polymers come in contact inside the die. The bilayer flow in the die wasalso simulated for entrance velocity of 3.0 cm/s for the cap layer, while keeping the entrance velocity for substrate to0.1 cm/s
For the three different combinations of LDPEA and LDPED, as well as for the case with larger flow rate (LFR) throughthe cap layer, Fig. 5 shows the predicted interface shape between the two layers. In Fig. 5, all four interface profileslook very similar, except for the interface shape in Fig. 5 (b). In Fig. 5 (b), the interface shape near the contact line inthe vertical tab on the left where the cap layer wraps around the substrate is quite different than the interface shapefor the other three cases. This difference in the interface shape for the case with higher viscosity polymer (LDPED) inthe cap layer and lower viscosity polymer (LDPEA) in the substrate is further clarified in Fig. 6. When the viscosity ofthe polymer in the cap layer is the same (Fig. 6 a, d) or lower (Fig. 6 c) than the viscosity for the polymer in thesubstrate, after the two polymers come in contact at the contact line, the interface between the two layers goestowards the exit along the axial direction. However, for the case with higher viscosity polymer in the cap layer (Fig. 6b), in the vertical tab on the left where the cap layer wrap around the substrate, the interface first goes toward theentrance before reversing back and starting to move toward the exit. It was confirmed that for this case with thehigher viscosity polymer in the cap layer, the polymer velocity in this region near the vertical tab is in fact towards theentrance. Because of this initial movement of the interface towards the entrance, for the case with the higher viscositypolymer (LDPED) in the cap layer, the vertical tab on the left is almost completely occupied by the higher viscosity
polymer (green line in Fig. 7). That is, for this case there is almost no substrate polymer in the vertical tab. For thehorizontal wall on top of the extrudate profile, effect of the polymer viscosity on the interface location at the die exit isshown in Fig. 7 (b). Effect of viscosity on the interface location in the horizontal wall can be explained by examining thevelocity distributions shown in Fig. 8. In comparison to the case with low viscosity polymer (LDPEA) in the substrateas well as the cap layer (Fig. 8 a), for the case with higher viscosity polymer (LDPED) in the cap layer (Fig. 8 b), thevelocity of the polymer in the cap layer is lower at the die exit. Therefore, in Fig. 7 (b) in order to satisfy the massbalance, the interface in the horizontal wall at the die exit is lower for this case (green line). In contrast, for the casewith higher viscosity polymer (LDPED) in the substrate and the lower viscosity polymer (LDPEA) in the cap layer, asexpected, the velocity in Fig. 8 (c) is higher in the cap layer. Therefore, in order to satisfy the mass balance, theinterface for this case is located at the highest position in Fig. 7 (b) (blue line). That is, the cap layer is the thinnest forthis case. It is evident from Fig 7 (a) that the cap layer for this case may be too thin in the region where the verticaltab on the left connects with the horizontal wall. In this region where the vertical tab is joined with the horizontal wall,for the case with higher viscosity polymer (LDPED) in the substrate, the interface is almost touching the die wall. Thatis, for this case there may not be any cap layer in this region where the vertical tab connects with the horizontal wall.For the last case with LDPEA in the substrate as well as the cap layer, but larger (double) flow rate in the cap layer,(Fig. 8 d, and black line in Fig 7), as expected, the interface is lower in comparison to the case with smaller velocity inthe cap layer and with LDPEA in both layers (red line in Fig. 7).
For the three cases with different polymer combinations and the case with larger flow rate (LFR) through the cap layer,the velocity distribution at the die exit and the velocity distribution in the plane where the cap layer first comes incontact with the substrate are shown in Fig. 9. It should be noted that the range of scale bars in Fig. 8 and Fig. 9 aredifferent. For all four cases, the flow in the substrate is not very well balanced. In particular, the velocity is significantlyhigher in the vertical wall connecting the circle in the middle with the bottom horizontal wall. This higher velocity in thevertical wall can be easily reduced, that is, the floor at the die exit can be easily balanced, by reducing the opening inthis region in the die plates between the circular entrance and the final die plate at the exit.
Fig. 10 shows the pressure distributions for the four coextrusion simulations in the profile die. As expected, thepressure is zero at the exit, and because of its smaller crosssection and higher velocity, the pressure is the highest inthe circular channel at the entrance of the cap layer. In comparison to the pressure for the case with LDPEA in bothlayers, the pressure in the die increases when the higher viscosity polymer (LDPED) is used in the substrate (Fig. 10c) or in the cap layer (Fig. 10 b). Also, the pressure in the two distribution channels and the circular entrance channelincreases for the case with larger flow rate in the cap layer (Fig. 10 d).
The shear rate on the die walls for the four coextrusion simulations is shown in Fig. 11. For all four cases the shear rateis the highest in the cap layer in the plane where it meets the substrate for the first time. Also, it is noted that after thetwo polymers meet, the shear rate in the cap layer is higher for the case with the higher viscosity polymer (LDPED) inthe substrate (Fig. 11 c) because after the two polymers meet the velocity in the cap layer is higher for this case (seeFig. 8 c). For the case with higher velocity through the cap layer (Fig. 11 d), as expected, the shear rate is higher inthe narrow channel connecting the two distribution channels for the cap layer and in the narrow channel connecting thesecond distribution channel with the contact line where the two polymers meet.
Fig. 12 shows the residence time distributions for the polymers in the substrate and the cap layer. In Fig. 12, for thefour coextrusion simulations, the residence time for the substrate is much larger than the residence time for the caplayer. The larger residence time for the substrate is expected because the circular entrance channel for the substratehas a larger crosssectional area. Accordingly, a smaller velocity (1 mm/s) was specified at the entrance of the circularentrance channel for substrate, whereas a much higher velocity (1.5 cm/s or 3.0 cm/s) was specified at the entrance ofthe circular entrance channel for cap layer. Also, as expected, the residence time for the cap layer is smaller for thecase with larger flow rate through the cap layer (black line with square symbol in Fig. 12). For the three cases withdifferent polymer combinations in the substrate and the cap layer, even though the residence time distribution for thecap layer (and also for substrate) are different for different polymer combinations, the difference in the residence timefor the cap layer (and also for substrate) for the three cases is small, and is probably within the accuracy of thepredictions. That is, for the three different polymer combinations, viscosities of the polymers seem to have only aminor effect on the residence time distribution.
ConclusionsMesh partitioning technique was used for simulation of a bilayer coextrusion in a complex profile die. Since the meshpartitioning technique does not require the interface between different polymer layers to match with the interelementboundaries (instead, allowing the interface to cut through the tetrahedral finite elements), this technique could be usedto simulate the flow in a highly complex bilayer coextrusion die. Effect of polymer viscosity on interface shape,velocity, pressure, shear rate, and residence time distribution was analyzed. Viscosities of the two polymers were foundto have significant effect on the interface shape, velocity, pressure, and shear rate in the die, but only a minor effecton the residence time distributions of the two polymers.
References 1. C. Rauwendaal, “Polymer Extrusion”, Hanser Publishers, New York (1994). 2. A. Karagiannis, A. N. Hyrmak, and J. Vlachopoulos, Rheologica Acta, Vol. 29, 71 – 87 (1990).
3. PolyXtrue software, Plastic Flow, LLC, Houghton, MI, 49931. 4. J. Dheur and M. J.Crochet, Rheologica Acta, Vol. 26, 401 – 413 (1987).
5. M. Gupta, SPE ANTEC Technical Papers, Vol. 54, 217 – 222 (2008). 6. J. Dooley and L. Rudolph, Journal of Plastic Film and Sheeting, Vol. 19, 111 – 123 (2003).
Return to Paper of the Month.